asphalt mixes produced with asphalt shingle ?· asphalt mixes produced with asphalt shingle sand...
Post on 21-Oct-2018
Embed Size (px)
Asphalt Mixes Produced with Asphalt Shingle Sand
Frdric Nel, ing. Deputy Technical Director
Sintra Inc. Montreal, Quebec
Jean-Martin Croteau, P. Eng.
Technical Director Colas Canada Inc. St. Albert, Alberta
Canadian Technical Asphalt Association 2015
452 ASPHALT MIXES PRODUCED WITH ASPHALT SHINGLE SAND
The use of RAS particles obtained from grinding/shredding of asphalt shingles is currently limited to between 3 and 5 percent. The addition of the sand only portion of RAS can reach more than 10 percent or even 15 percent while providing rheological characteristics different enough from those of conventional HMA. The technique is to sieve the shredded RAS particles to separate the fibres/bitumen clusters from the sand component. Only the shingle sand is recycled to the mix to facilitate obtaining a completely homogeneous mixture. The formulation of HMA containing a high RAS sand content is based on characterizing the mechanical properties of the HMA. HMA modified with high RAS sand content have a total bitumen content of about 8 percent. This paper discusses the characterization of the mechanical properties of HMA modified with RAS sand and the advantages of this technique. It was determined that rutting, thermal cracking and asphalt module were close to values normally obtained for the same formulation without recycling. On the other hand, there is a significant difference in fatigue resistance which is increased compared to conventional HMA.
La limite actuelle de recyclage de bardeau incorpor sous de particules issues dun broyage/dchiquetage est de 3.0 5.0 %. Lincorporation de la partie sable du bardeau dasphalte seulement permet des teneurs en recyclage suprieures 10 %, voire 15 % tout en offrant des caractristiques rhologiques assez diffrentes de celles des enrobs classiques.
La technique consiste cribler les particules de bardeau dchiquetes pour sparer les agglomrations fibres/bitume de la composante sable. Seul le sable de bardeau est recycl dans lenrob pour favoriser lobtention dun mlange compltement homogne. La formulation des enrobs incorporant un forte teneur en sable de bardeau est base sur une caractrisation des proprits mcaniques des enrobs. Les formules denrobs modifis au sable de bardeau ont des teneurs totales en bitume de lordre de 8 %.
Cet article prsente comment la caractrisation des proprits mcaniques de formulation denrobs ainsi modifis a permis de dmontrer les avantages de cette technique. Il a t dtermin que lornirage, la fissuration thermique et le module de lenrob taient proche des valeurs normalement obtenue pour la mme formulation sans recyclage. L o il y a une diffrence significative, cest la rsistance la fatigue qui est augment par rapport aux enrobs classiques.
Canadian Technical Asphalt Association 2015
NOL & CROTEAU 453
Flexible pavements have several layers: sub-base, base, binder course, and surface course. Those pavement layers commonly comprise granular materials in the lower layers and asphalt-bound materials in the upper layers. Asphalt-bound materials are a mixture of various aggregate fractions, i.e., aggregate, sand and filler, and an asphalt binder.
The binder may be a new binder consisting of neat or modified asphalt obtained from the petroleum industry. The new binder may contain various additives, such as polymers or elastomers that modify its viscoelastic properties. For reasons of economy and to meet environmental requirements, the binder used in asphalt mixes may also consist of a mixture of binders obtained from recycled materials an old binder and a new binder as described above, hereinafter called a virgin binder.
It is in fact common practice to use, in the production of asphalt paving materials, recycled asphalt materials originating from degraded asphalt pavement. Those reclaimed materials are then crushed and screened to obtain a homogeneous gradation. The recycled asphalt materials thus produced are called Reclaimed Asphalt Pavement; commonly known as RAP.
Using RAP in asphalt mixes is a standard practice in most European countries  and in North America, where its use has been incorporated in the Superpave volumetric mix design system . The RAP commonly available has an average composition similar to that of asphalt mixes produced and applied as paving materials, i.e., an average asphalt content by weight of 4 to 6 percent relative to total weight of RAP, with the rest of the composition being a mineral mix of coarse aggregate, sand and filler.
The asphalt binder contained in RAP has undergone an aging process during production and placement, and then progressively in place, due to oxidation and chemical evolution. Aging of asphalt binder is the result of volatile elements being lost, causing hardening of the binder. The hardening of the binder may be measured by simply comparing the RAP binders rheological properties to those of the original binder. Thus, the binder of RAP originating from pavement located in a geographical area where the common binder is PG 58-28 grade may have hardened to a PG 70-16, or even harder binders.
More recently, Reclaimed Asphalt Shingles (RAS) have been used as recycled asphalt materials . Reclaimed asphalt shingle originates either from batches of defective asphalt shingles rejected during manufacturing or from asphalt shingles removed from old roofs during roofing repairs. For example, it is estimated that between 150,000 and 200,000 tonnes of old asphalt roofing shingles are landfilled in Quebec at a cost of $25 to $30 per tonne every year. Once debris (e.g., wood, nails, etc.) has been removed, the shingles are finely shredded and screened into RAS to facilitate their incorporation into asphalt mixes.
The RAS generally contain 20 to 30 percent by weight of asphalt, 25 to 30 percent of fine mineral filler, 30 to 35 percent of mineral aggregates, and 5 to 10 percent of glass or cellulose fibres. Recycling shingles in asphalt mixes closely resembles RAP recycling. Thus, the aggregate in asphalt shingles makes it possible to use less aggregate when developing the final asphalt mix and the shingles asphalt also makes it possible to use less virgin binder when manufacturing the final asphalt mix. Accordingly, the greater the shingle content, the less virgin binder required.
However, the RAS asphalt binder is different from the asphalt binder contained in RAP; it is generally much harder than asphalt binder used in road applications. Given that the asphalt binder in RAS is hard, the asphalt mix containing RAS and less virgin/soft binder may become more brittle. In addition, the
Canadian Technical Asphalt Association 2015
454 ASPHALT MIXES PRODUCED WITH ASPHALT SHINGLE SAND
density of shingles is relatively low which makes it difficult to obtain good density for an asphalt mixture. As a result, the addition of RAS in asphalt mixes is generally limited to 5 percent and the binder consideration from the shingle limited to 40 percent in Quebec. Incidentally, if the rate of recycling of RAS is 5.0 percent, the asphalt binder content of shingles is 25 percent, and 40 percent of that binder is available as mixing binder for the asphalt mixture, the rate of virgin binder for the asphalt mixture may be reduced by 0.5 percent. Beyond that, it is recognized that the asphalt mix may become lean in binder and more brittle.
There is a need to upgrade old asphalt shingles to produce an asphalt mix composition that avoids all or some of the disadvantages mentioned. In particular, it is desirable to provide an asphalt mix containing a substantial quantity of asphalt shingles, without modifying the mechanical and rheological properties of the asphalt mix, i.e., by ensuring that it is not brittle despite its high content of asphalt shingles.
Accordingly, the object of this paper is the evaluation of asphalt mixes produced with only shingle sand extracted from RAS. The shingle sand is obtained by screening out the fibre/bitumen flakes from the shredded asphalt shingles. The composition of the shingle sand obtained in this manner is 15 to 20 percent of asphalt binder, 80 to 85 percent of mineral aggregate with a top size aggregate less than 2.5 mm, and only traces of glass or cellulose fibres.
2.0 ASPHALT MIXES MODIFIED WITH ASPHALT SHINGLE SAND
The asphalt mix produced with RAS offers the advantage of reclaiming industrial waste. The commonly used RAS particles resulting from crushing/shredding asphalt shingles have a maximum size in the order of 12.5 mm. The asphalt mix produced according to the method proposed in this paper contains only the sand/filler fraction of asphalt shingles, i.e., it is free of particles larger than 2.5 mm and contains only trace amounts of glass or cellulose fibres.
To obtain shingle sand, the crude shingle particles undergo additional processing to separate the fibre/asphalt agglomerations from the shingle sand. Then, as opposed to the current shingle recycling practice, only the shingle sand is recycled in the asphalt mix to obtain a fully homogenous asphalt mix with density comparable to conventional asphalt mixes.
Even at recycling proportions up to 15 percent, the use of shingle sand makes it possible to obtain a homogenous and dense asphalt mix composition with mechanical performance similar to that of conventional asphalt mixes. Whereas the incorporation of complete RAS, with fibre/asphalt agglomerations, adversely affects both the homogeneity and mix density of the final asphalt mix. This is why the common recycling rate of complete RAS is often limited to a maximum of 5 percent.
In addition, the specific gravity of asphalt sand may be evaluated to about the same as that o